Zintl Phase Variations Through Cation Selection. Synthesis and Structure of A21Cd4Pn18 (A = Eu, Sr, Ba; Pn = Sb, Bi)
Sheng-Qing Xia; Svilen Bobev; Inorganic Chemistry 47 (2008) 1919–1921; doi:10.1021/ic800242a

data_4305050
_publ_contact_author_address
; 
Department of Chemistry and Biochemistry
304A Drake Hall
University of Delaware
Newark, DE 19716
USA
;
_publ_contact_author_email       sbobev@chem.udel.edu
_publ_contact_author_fax         'Intl. Code + (302) 8316335'
_publ_contact_author_phone       'Intl. Code + (302) 8318720'
_publ_section_title
;
Zintl Phase Variations Through Cation Selection. Synthesis and Structure of
A21Cd4Pn18 (A = Eu, Sr, Ba; Pn = Sb, Bi)
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              1919
_journal_page_last               1921
_journal_paper_doi               10.1021/ic800242a
_journal_volume                  47
_journal_year                    2008
_chemical_formula_moiety         'Bi11 Cd4, 7(Bi), 21(Sr)'
_chemical_formula_sum            'Bi18 Cd4 Sr21'
_chemical_formula_weight         6051.26
_space_group_IT_number           12
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 92.064(4)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   18.510(5)
_cell_length_b                   17.685(4)
_cell_length_c                   18.213(4)
_cell_measurement_reflns_used    6290
_cell_measurement_temperature    120(2)
_cell_measurement_theta_max      26.37
_cell_measurement_theta_min      1.59
_cell_volume                     5958(2)
_computing_cell_refinement       'SMART (Bruker, 2000)'
_computing_data_collection       'SMART (Bruker, 2000)'
_computing_data_reduction        'SAINT (Bruker, 1999)'
_computing_molecular_graphics    'SHELXTL 5.1 (Sheldrick, 1994)'
_computing_publication_material  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      120(2)
_diffrn_detector_area_resol_mean 8.3
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device_type  'Bruker Smart APEX'
_diffrn_measurement_method       \w
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0855
_diffrn_reflns_av_sigmaI/netI    0.0636
_diffrn_reflns_limit_h_max       23
_diffrn_reflns_limit_h_min       -23
_diffrn_reflns_limit_k_max       22
_diffrn_reflns_limit_k_min       -22
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_limit_l_min       -22
_diffrn_reflns_number            31824
_diffrn_reflns_theta_full        26.37
_diffrn_reflns_theta_max         26.37
_diffrn_reflns_theta_min         1.59
_diffrn_standards_decay_%        0
_diffrn_standards_interval_count 0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    72.929
_exptl_absorpt_correction_T_max  0.077
_exptl_absorpt_correction_T_min  0.047
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS (Sheldrick, 2003)'
_exptl_crystal_colour            Black
_exptl_crystal_density_diffrn    6.746
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Irregular
_exptl_crystal_F_000             9936
_exptl_crystal_size_max          0.07
_exptl_crystal_size_mid          0.04
_exptl_crystal_size_min          0.04
_refine_diff_density_max         6.080
_refine_diff_density_min         -3.069
_refine_diff_density_rms         0.673
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.131
_refine_ls_matrix_type           full
_refine_ls_number_parameters     215
_refine_ls_number_reflns         6290
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.131
_refine_ls_R_factor_all          0.0642
_refine_ls_R_factor_gt           0.0519
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0344P)^2^+744.0148P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1146
_refine_ls_wR_factor_ref         0.1207
_reflns_number_gt                5279
_reflns_number_total             6290
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic800242a-file002_3.cif
_cod_data_source_block           Sr21Cd4Bi18
_cod_depositor_comments
;
The following automatic conversions were performed:
'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to '/home/saulius/struct/CIF-dictionaries/cif_core.dic'
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 
;
_cod_original_sg_symbol_H-M      'C 2/m'
_cod_database_code               4305050